| ||Format||Pages||Price|| |
|3||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$48.00||  ADD TO CART|
|Standard + Redline PDF Bundle||6||$56.00||  ADD TO CART|
This specification covers crushed steel slag coarse and fine aggregates suitable for use in bituminous paving mixtures. The coarse and fine aggregates shall consist of hard, tough, durable pieces of steel slag, and shall be processed, as necessary, by crushing or screening, or both, and magnetic separation for the removal of metallics. At the time of delivery, the aggregates shall not contain injurious amounts of foreign materials such as clay, loam, wood, tramp metal, unhydrated lime, or other deleterious materials. The physical requirements for which the aggregates shall be tested on and consequently conform to are grading and fineness modulus, polishing characteristics, soundness, degradation, expansion, friable particles, stripping, adherent coatings, crushed count, plasticity index, leaching; and environmental stability.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers crushed steel slag coarse and fine aggregates suitable for use in bituminous paving mixtures.
1.2 Steel slag coarse and fine aggregates are currently being used entirely ( ) or combined with other mineral aggregates, such as those covered in Specification or , to produce paving mixtures similar to those described in Specification or .
Note 1: When 100 % of the coarse aggregate in a bituminous mixture is steel slag, the amount of steel slag fines in that mixture may be limited to prevent bulking.
1.3 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
Note 2: Sieve size is identified by its standard designation in Specification . The alternative designation given in parentheses is for information only and does not represent a different standard sieve size.
1.4 The text of this specification references notes and footnotes which provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of the standard.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C88 Test Method for Soundness of Aggregates by Use of Sodium Sulfate or Magnesium Sulfate
C117 Test Method for Materials Finer than 75-m (No. 200) Sieve in Mineral Aggregates by Washing
C125 Terminology Relating to Concrete and Concrete Aggregates
C131 Test Method for Resistance to Degradation of Small-Size Coarse Aggregate by Abrasion and Impact in the Los Angeles Machine
C136 Test Method for Sieve Analysis of Fine and Coarse Aggregates
C142 Test Method for Clay Lumps and Friable Particles in Aggregates
D8 Terminology Relating to Materials for Roads and Pavements
D75 Practice for Sampling Aggregates
D448 Classification for Sizes of Aggregate for Road and Bridge Construction
D692 Specification for Coarse Aggregate for Bituminous Paving Mixtures
D1073 Specification for Fine Aggregate for Bituminous Paving Mixtures
D3319 Practice for the Accelerated Polishing of Aggregates Using the British Wheel
D3515 Specification for Hot-Mixed, Hot-Laid Bituminous Paving Mixtures
D3665 Practice for Random Sampling of Construction Materials
D4215 Specification for Cold-Mixed, Cold-Laid Bituminous Paving Mixtures
D4318 Test Methods for Liquid Limit, Plastic Limit, and Plasticity Index of Soils
D4792 Test Method for Potential Expansion of Aggregates from Hydration Reactions
D4867/D4867M Test Method for Effect of Moisture on Asphalt Concrete Paving Mixtures
D5711 Test Method for Determining the Adherent Coating on Coarse Aggregates
D5821 Test Method for Determining the Percentage of Fractured Particles in Coarse Aggregate
E11 Specification for Woven Wire Test Sieve Cloth and Test Sieves
ICS Number Code 91.100.15 (Mineral materials and products)
UNSPSC Code 30111802(Artificial aggregate); 30121500(Bituminous derivatives)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D5106-15, Standard Specification for Steel Slag Aggregates for Bituminous Paving Mixtures, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top